Near-infrared emitting CdTe0.5Se0.5/Cd0.5Zn0.5S quantum dots: synthesis and bright luminescence
© Yang et al.; licensee Springer. 2012
Received: 1 September 2012
Accepted: 21 October 2012
Published: 6 November 2012
We present how CdTe0.5Se0.5 cores can be coated with Cd0.5Zn0.5S shells at relatively low temperature (around 200°C) via facile synthesis using organic ammine ligands. The cores were firstly fabricated via a less toxic procedure using CdO, trioctylphosphine (TOP), Se, Te, and trioctylamine. The cores with small sizes (3.2-3.5 nm) revealed green and yellow photoluminescence (PL) and spherical morphologies. Hydrophobic core/shell CdTe0.5Se0.5/Cd0.5Zn0.5S quantum dots (QDs) with tunable PL between green and near-infrared (a maximum PL peak wavelength of 735 nm) were then created through a facile shell coating procedure using trioctylphosphine selenium with cadmium and zinc acetate. The QDs exhibited high PL efficiencies up to 50% because of the formation of a protective Cd0.5Zn0.5S shell on the CdTe0.5Se0.5 core, even though the PL efficiency of the cores is low (≤1%). Namely, the slow growth process of the shell plays an important role for getting high PL efficiencies. The properties of the QDs are largely determined by the properties of CdTe0.5Se0.5 cores and shells preparation conditions such as reaction temperature and time. The core/shell QDs exhibited a small size diameter. For example, the average diameter of the QDs with a PL peak wavelength of 735 nm is 6.1 nm. Small size and tunable bright PL makes the QDs utilizable as bioprobes because the size of QD-based bioprobes is considered as the major limitation for their broad applications in biological imaging.
KeywordsQuantum dots Semiconductor Photoluminescence Near-infrared Core/shell
Semiconductor quantum dots (QDs) have attracted considerable interest in the past decade because of their excellent properties such as narrow, symmetric, and tunable emission spectra, broad absorption spectra, superior photostability, high photoluminescence (PL) efficiency, and the capacity of simultaneous excitation of multiple fluorescence colors compared with the organic dyes and fluorescent proteins [1–4]. Moreover, the near-infrared (NIR) spectral range presents many advantages for in vivo fluorescence imaging. The absorption of photons by biological tissues is much reduced in this spectral window compared with the visible range. There are many more alternatives in QDs with NIR emission for in vivo imaging than organic dyes . For example, the QDs with a PL of 700-nm region minimize the problems of indigenous fluorescence of tissues and meet the requirements of in vivo biological imaging applications. Therefore, the synthesis of NIR-emitting QDs (700–900 nm) has received much attention recently. In addition, the QDs have advantages compared with metallic nanoparticles for nanoprobes because of their broad absorption band and tunable and bright PL .
CdSe is still one of the most popular QDs created by various chemical strategies. However, CdSe (Eg = 1.76 eV, aB = 9.6 nm) QDs can be tuned through quantum confinement to emit visible fluorescent spectrum only reaching typically 650–700 nm. Furthermore, it is difficult to grow CdSe-based QDs with NIR emission because of their growth kinetics. In addition, the size of CdSe with a longer PL peak wavelength becomes too large for bioprobers. Compared with CdSe, the band gap of bulk CdTe is narrow (1.56 eV, corresponding to approximately 795 nm wavelength). The PL peak wavelength of CdTe QDs with a diameter of 7 nm can reach approximately 720 nm. However, CdTe and CdTe/CdSe QDs prepared by an organic synthesis are normally unstable, which results in low PL efficiency and fast photobleaching. Therefore, composited CdTe and CdSe QDs or CdTe-based QDs with protective inorganic shells are expected. Especially, these QDs with NIR emission and small size are necessary. However, there have been few reports of a higher band gap shell growth around CdTe or CdTeSe QDs. Rogach and co-workers described the aqueous synthesis of 8–10 nm CdTe-based QDs emitting at approximately 800 nm .
For a purpose of getting a highly stable fabricating CdTeSe-composited cores with a higher band gap shell is still a challenge. Nanoalloying of two semiconductors shows properties distinct not only from the properties of their bulk counterparts (such as CdTe0.5Se0.5), but also from those of their parent semiconductors (such as CdTe or CdSe). Engineering the band gap energy of QDs has resulted in the development of core/shell QDs with novel exciting properties and applications. Recently, Jiang et al. reported that they were able to deposit only a very thin CdS shell (approximately one monolayer) on the surface of a CdTeSe core . However, the band gap of CdS is not large enough to provide the potential barrier necessary to block both electrons and holes inside CdTeSe cores. A ZnS shell has a crucial role in the improvement of PL properties of QDs. This increases the chemical stability and photostability of the QDs because ZnS is a chemically stable with wide band gap (3.8 eV for the bulk material) semiconductor material. However, the large mismatch between CdTeSe and ZnS lattice parameters enables the strain at the interface between the core and the shell. Therefore, a Cd x Zn1−xS composite shell can also improve the stability and PL properties of the QDs. Very recently, we fabricated CdSe cores coated with Cd x Zn1−xS composite shells . These core/shell QDs reveal broadly tunable PL spectra (PL peak wavelength up to 650 nm), narrow size distribution, high PL efficiency (up to 60%, in the case of CdSe cores with a PL efficiency of 1%), and a high stability (keeping their initial PL efficiency in a toluene solution for 1 year).
To reduce the lattice parameter mismatch and improve the properties of core/shell QDs, an interlayer is inserted, such as CdS and ZnSe between the CdSe core and ZnS shell. A Cd x Zn1−xS composite shell has led to the formation of CdS interlayer due to the growth kinetics of CdS and ZnS. Thus, CdTeSe cores would strongly benefit from Cd x Zn1−xS composite shells for getting a longer PL peak wavelength, as well as high stability and PL efficiency. However, very little reports focused on the NIR emission of composite cores coated with a higher band gap composited shell. Recently, Pons et al. reported that near-infrared-emitting CdTeSe/CdZnS core/shell QDs prepared using cadmium oxide (CdO), zinc oxide (ZnO), tetradecylphosphonic acid (TDPA), cadmium oleate (Cd(OA)2), and zinc oleate (Zn(OA)2) as precursors revealed a high stability . Because of decreased lattice mismatch between the core and the shell, the interface strain decreases dramatically during the shell growth, indicating that the spatial distribution of defects in core/shell QDs can be controlled by the shell growth. A better understanding of the shell effect on optical properties of QDs is important for optimizing the synthesis. Because Cd-based QD is undesirable for biological imaging due to toxicity, a CdZnS shell with a ZnS-rich layer coated on the surface of CdSe is used to decrease the release of Cd ions in this paper. We further have a technique of glass coating on the surface of the QDs as well for the purpose of drastically reducing the amount of Cd released from the QDs as demonstrated in the previous publications [11, 12].
For the preparation of QDs by classical colloidal chemistry, organometallic and/or metal organic compounds under anaerobic conditions have been employed. For example, CdSe QDs were prepared by reacting dimethylcadmium (CdMe2) with trioctylphosphine selenium (TOP)Se in TOP/trioctylphosphine oxide or TOPO at high temperature . Therefore, a novel and facile synthesizing strategy, which uses a faster reaction process and less toxic chemicals, is highly desirable. To address a novel method for fabricating QDs with NIR PL, more efforts to other potential preparation methods of QDs have been taken in our group. In this paper, CdTe0.5Se0.5/Cd0.5Zn0.5S core/shell QDs were fabricated using less toxic chemicals and a facile synthesis. These core/shell QDs revealed tunable PL peak wavelength from the initial value of CdTe0.5Se0.5 cores to 735 nm with much improved PL efficiency above 50%. A detailed consideration allows us to grow multilayer Cd0.5Zn0.5S shell around CdTe0.5Se0.5 QDs using air stable zinc and cadmium acetate precursors at relatively low temperature (approximately 200°C). The resulting core/shell QDs exhibit improved stability and PL efficiency compared with CdTe/Cd0.5Zn0.5S QDs.
All chemicals were of analytical grade or of the highest purity available and used directly without any further purification. Cadmium oxide (CdO, 99.99%), cadmium acetate dihydrate (Cd(Ac)22H2O, 98%), zinc acetate (Zn(Ac)2, 99.99%), selenium (Se, 99.5%), sulfur (S, 99.98%, powder), tellurium (Te, 99.99%), octadecylphosphonic acid (ODPA, 97%), trioctylamine (TOA, 98%), octadecene (ODE, technical grade of 90%, ODE), TOP (97%), hexadecylamine (HDA), and TOA were supplied by Sigma Aldrich (St. Louis, MO, USA). The pure water was obtained from a Milli-Q synthesis system (resistivity of 18.2 MΩ·cm) (EMD Millipore Corporation, Billerica, MA, USA).
Preparation of CdTe0.5Se0.5, CdSe, and CdTe cores
Preparation conditions and properties of CdTe 0.5 Se 0.5 cores and CdTe 0.5 Se 0.5 /Cd 0.5 Zn 0.5 S core/shell QDs
Reaction time (min)
Reaction temperature (°C)
PL peak wavelength (nm)
PL efficiency (%)
Alternatively, CdSe cores were fabricated by injecting 1 mL of TOPSe with 1 mmol Se in the precursor of Cd within 30 s under N2 flow. After further reaction for 2 min, the resulting sample was separated by using a similar procedure with that of CdTe0.5Se0.5 cores. CdTe cores were synthesized by addition of 1 mL of TOPTe with 1 mmol Te within 30 s under N2 flow. The CdTe cores were precipitated twice in ethanol and resuspended in 10 mL of toluene.
Preparation of CdTe0.5Se0.5 and CdTe cores coated with Cd0.5Zn0.5S shell
The preparation of Cd0.5Zn0.5S shell was carried out by directly reacting cadmium and zinc acetate with TOPS. In a typical synthesis, 14 mg of Cd(Ac)22H2O, 10 mg of Zn(Ac)2, 0.5 g of HDA, and 5 mL of ODE were mixed in a three-neck round-bottom flask under N2 flow and stirred at 200°C until the Cd and Zn salts were completely dissolved. A 6 mg of S powder was dissolved in 0.5 mL of TOP. The toluene solution of CdTe0.5Se0.5 or CdTe cores (3 mL) was injected with vigorous stirring followed by the injection of the TOPS solution. The mixture was kept at 200°C with stirring for several to several 10 min, followed by cooling down to room temperature. The products were precipitated, washed twice with ethanol, and re-dispersed in 10 mL of toluene. To investigate the effect of preparation conditions on properties, reaction time and temperature were adjusted.
The transmission electron microscopy (TEM) observations of samples were performed mainly using a Hitachi EF-1000 electron microscope (Hitachi Ltd., Tokyo, Japan). The absorption and PL spectra were recorded using conventional spectrometers (Hitachi U-4000 and F-4500, respectively). Both excitation and emission slits are 5 nm for the measurement of PL spectra. The PL efficiencies of samples in solution were estimated using a method previously reported . Briefly, the PL and absorption spectra of a standard quinine solution (quinine in 0.1 N H2SO4 solution; PL efficiency η0 of 55%) were measured in a 1-cm quartz cell as a function of the concentration.
Results and discussion
where d is the QD diameter and a and c are empirical fit parameters. Since the PL properties of QDs depended strongly on their band gap and size, the alloyed CdTe0.5Se0.5 QDs revealed different PL properties compared with CdTe and CdSe QDs.
Property comparison of CdTe, CdSe, and CdTe 0.5 Se 0.5 QDs
PL peak wavelength (nm)
Preparation condition and properties of CdTe 0.5 Se 0.5 /Cd 0.5 Zn 0.5 S QDs
Preparation condition and properties of CdTe 0.5 Se 0.5 /Cd 0.5 Zn 0.5 S QDs
Because CdSe/CdS QDs have less lattice mismatch (approximately 3.9%) than that of CdSe/ZnS QDs (approximately 12%) [18, 19], an alloy Cd x Zn1−xS shell can provide better stability by decreasing interfacial strain between cores and shells. Quyang et al. reported that gradiently alloyed Zn x Cd1−xS QDs having a Cd-rich core and Zn-rich shell could be synthesized via a noninjection one-pot approach . In our experiments CdTe0.5Se0.5 cores were coated with Cd0.5Zn0.5S composite shell by an organic one-step synthesis. The shell layers of CdS and ZnS might not be clearly separated, and it is also possible that the shell layer is a gradient alloy structure of CdS and ZnS. This is ascribed to the growth kinetic of CdS and ZnS. The gradient structure would be beneficial to improve stability by reducing lattice mismatch between CdSe and ZnS layers.
According to our previous experimental results, an optimal molar ratio of Cd/Zn of 1/1 was used for CdTe0.5Se0.5 cores coated with Cd0.5Zn0.5S shell for getting high PL efficiencies. To investigate the effect of temperature on the formation of Cd0.5Zn0.5S shell on CdTe0.5Se0.5 cores, reaction temperature was adjusted from 180°C to 280°C. An optimal temperature range was found to be around 190°C to 220°C. In the case of a high temperature (more than 260°C), the reaction solution became black quickly when TOPS was injected. This is ascribed to the PL quenching of QDs because the high temperature led to large amount defects generated during preparation. Table 1 summarizes the preparation conditions and properties of CdTe0.5Se0.5 cores and CdTe0.5Se0.5/Cd0.5Zn0.5S QDs.
For traditional QD synthesis by organic amine as a capping agent, researchers normally selected metal oleate and stearate as precursors. The combination of precursor and ligand is important for the non-coordinating solvent system. Metal stearate is a relatively stable precursor that could be coheated with a higher ratio of alkylamines such as 1-octadecylamine and HDA at high temperature (280°C-320°C) . In contrast nucleation and growth in a metal oleate and HDA reaction system are executed at a moderate reaction temperature (265°C-285°C). In the present experiments, CdTe0.5Se0.5 cores were coated with Cd0.5Zn0.5S shells using cadmium and zinc acetate as precursors to react with TOPS in ODE with HDA. The reaction temperature can be further lowered because of salt acetate with a short carbon chain. In addition the preparation of the core/shell QDs has to be carried out quickly to prevent the decomposition of salt acetate. Namely, cadmium and zinc acetate can be decomposed into CdO and ZnO if the solution was kept at a high temperature (more than 240°C) for a long time (more than 20 min). In contrast the reaction for the formation of QDs can be easily controlled at low temperature (less than 210°C). Because of a slow growth procedure, the core/shell QDs revealed a high PL efficiency as shown in Table 1.
The PL efficiency of QDs is significantly influenced by the QDs’ surface state, such as the stoichiometric ratio of anion and cation, the nature and coverage ratio of the capping agent, and the polarity of the dispersing solvent . In order to stabilize and maximize PL, a semiconductor shell with higher band gap not only passivates the surface bonds but also varies the semiconductor potential energy well, concentrating the charge carriers in a core away from the surface [22, 23]. Thereby, surface defect states and trap sites will have a diminished impact on the PL efficiency, and fewer environmental factors will influence the emission intensity. At the beginning of a shell coating, the passivation of a surface led a quick increase of PL efficiency. When the shell grew to a desired thickness, the corresponding PL efficiency of the resulting core/shell QDs approached the maximum value.
Generally, CdTe QDs show poor photostability because of the easy oxidation of tellurium as we have mentioned before. The stability was increased by being coated with a Zn0.5Cd0.5S shell. Especially in the case of CdTe0.5Se0.5 cores coated with a Cd0.5Zn0.5S shell, the core/shell QDs with a QD concentration of 100 nM in a toluene solution retained their initial PL efficiency for 1 month.
A successful approach for preparing highly luminescent CdTe0.5Se0.5/Cd0.5Zn0.5S core/shell QDs has been presented. CdSe, CdTe, and CdTe0.5Se0.5 cores were first fabricated by a less toxic organic synthesis. Experimental results indicated that the size and PL properties depended strongly on the injection speed of anion precursors. CdSe and CdTe0.5Se0.5 cores exhibited high stability, while the PL of CdTe cores was quenched after 2 days. Subsequently, CdTe0.5Se0.5 cores were coated with Cd0.5Zn0.5S shells at relatively low temperature by using metal acetate and TOPS. This method has significant advantages: being less toxic, insensitive to air and moisture, easier to purify, and provide highly monodispersed QDs with a high PL efficiency and NIR emission. Namely, the Cd0.5Zn0.5S shell makes a CdTe0.5Se0.5 core a significant red shift of both absorption and PL spectra with reaction time. Experimental results indicated that the lower deposition temperature played a critical role for overgrowing shell material around the cores and getting high PL efficiency of the core/shell QDs. The emission wavelength from the core/shell QDs can span from the initial PL of the CdTe0.5Se0.5 core to 735 nm, which is achieved through the construction of the structure of a composite shell on a composite core. Because of tunable PL wavelength, high PL efficiency, and high stability, we expect that these core/shell QDs would be promising biomedical fluorophores for ultrasensitive, multicolor, and multiplexing applications, especially in vivo biomedical imaging applications.
- Somers RC, Bawendi MG, Nocera DG: CdSe nanocrystal based chem-/bio-sensors. Chem Soc Rev 2007, 36: 579–591. 10.1039/b517613cView ArticleGoogle Scholar
- Tessler N, Medvedev V, Kazes M, Kan SH, Banin U: Efficient near-infrared polymer nanocrystal light-emitting diodes. Science 2002, 295: 1506–1508. 10.1126/science.1068153View ArticleGoogle Scholar
- Peng L, Wang Y, Dong Q, Wang Z: Passivated ZnSe nanocrystals prepared by hydrothermal methods and their optical properties. Nano-Micro Lett 2010, 2: 190–196.View ArticleGoogle Scholar
- Wu J, Wang ZM, Dorogan VG, Li S, Mazur YI, Salamo JG: Nanoscale, near infrared broadband emission of In0.35Ga0.65As quantum dots on high index GaAs surfaces. Nanoscale 2011, 3: 1485–1488. 10.1039/c0nr00973cView ArticleGoogle Scholar
- Gao J, Chen K, Xie R, Xie J, Yan Y, Cheng Z, Peng X, Chen X: In vivo tumor-targeted fluorescence imaging using near-infrared non-cadmium quantum dots. Bioconjugate Chem 2010, 21: 604–609. 10.1021/bc900323vView ArticleGoogle Scholar
- Karthick Raja Namasivayam S, Gnanendra Kumar E, Reepika R: Synthesis of silver nanoparticles by Lactobaciluus acidophilus 01 strain and evaluation of its in vitro genomic DNA toxicity. Nano-Micro Lett 2010, 2: 160–163.View ArticleGoogle Scholar
- Rogach AL, Franzl T, Klar TA, Feldmann J, Gaponik N, Lesnyak V, Shavel A, Eychmuller A, Rakovich YP, Donegan JF: Aqueous synthesis of thiol-capped CdTe nanocrystals: state-of-the-art. J Phys Chem C 2007, 111: 14628–14637. 10.1021/jp072463yView ArticleGoogle Scholar
- Jiang W, Singhal A, Zheng J, Wang C, Chan WCW: Optimizing the synthesis of red- to near-IR-emitting CdS-capped CdTexSe1−x alloyed quantum dots for biomedical imaging. Chem Mater 2006, 18: 4845–4854. 10.1021/cm061311xView ArticleGoogle Scholar
- Yang P, Ando M, Taguchi T, Murase N: Highly luminescent CdSe/CdxZn1−xS QDs with narrow spectrum and widely tunable wavelength. J Phys Chem C 2011, 115: 14455–14460. 10.1021/jp201214kView ArticleGoogle Scholar
- Pons T, Lequeux N, Mahler B, Sasnouski S, Fragola A, Dubertret B: Synthesis of near-infrared-emitting, water-soluble CdTeSe/CdZnS core/shell quantum dots. Chem Mater 2009, 21: 1418–1424. 10.1021/cm8027127View ArticleGoogle Scholar
- Yang P, Murase N, Suzuki M, Hosokawa C, Kawasaki K, Kato T, Taguchi T: Bright, non-blinking, and less-cytotoxic SiO2 beads with multiple CdSe/ZnS nanocrystals. Chem Commun 2010, 46: 4595–4597. 10.1039/c002243hView ArticleGoogle Scholar
- Yang P, Ando M, Murase N: Highly luminescent CdSe/CdxZn1−xS quantum dots coated with thickness-controlled SiO2 shell through silanization. Langmuir 2011, 27: 9535–9540. 10.1021/la201213cView ArticleGoogle Scholar
- Sheng W, Kim S, Lee J, Kim SW, Jensen K, Bawendi MG: In-situ encapsulation of quantum dots into polymer microspheres. Langmuir 2006, 22: 3782–3790. 10.1021/la051973lView ArticleGoogle Scholar
- Murase N, Li C: Consistent determination of photoluminescence quantum efficiency for phosphors in the form of solution, plate, thin film, and powder. J Lumin 2008, 128: 1896–1903. 10.1016/j.jlumin.2008.05.016View ArticleGoogle Scholar
- Zeng Q, Kong X, Sun Y, Zhang Y, Tu L, Zhao J, Zhang H: Synthesis and optical properties of type II CdTe/CdS core/shell quantum dots in aqueous solution via successive ion layer adsorption and reaction. J Phys Chem C 2008, 112: 8587–8593. 10.1021/jp711395fView ArticleGoogle Scholar
- Regulacio MD, Han M: Composition-tunable alloyed semiconductor nanocrystals. Acc Chem Res 2010, 43: 621–630. 10.1021/ar900242rView ArticleGoogle Scholar
- Swafford LA, Weigand LA, Bowers MJ II, McBride JR, Rapaport JL, Watt TL, Dixit SK, Feldman LC, Rosenthal SJ: Homogeneously alloyed CdSxSe1−x nanocrystals: synthesis, characterization, and composition/size-dependent band gap. J Am Chem Soc 2006, 128: 12299–12306. 10.1021/ja063939eView ArticleGoogle Scholar
- Zhong XH, Feng YY, Knoll W, Han MY: Alloyed ZnxCd1−xS nanocrystals with highly narrow luminescence spectral width. J Am Chem Soc 2003, 125: 13559–13563. 10.1021/ja036683aView ArticleGoogle Scholar
- Talapin DV, Mekis I, Götzinger S, Kornowski A, Benson Q, Weller H: CdSe/CdS/ZnS and CdSe/ZnSe/ZnS core-shell-shell nanocrystals. J Phys Chem B 2004, 108: 18826–18831. 10.1021/jp046481gView ArticleGoogle Scholar
- Ouyang JY, Ratcliffe CI, Kingston D, Wilkinson B, Kuijper J, Wu XH, Ripmeester JA, Yu K: Gradiently alloyed ZnxCd1−xS colloidal photoluminescent quantum dots synthesized via a noninjection one-pot approach. J Phys Chem C 2008, 112: 4908–4919. 10.1021/jp710852qView ArticleGoogle Scholar
- Sun M, Yang X: Phosphine-free synthesis of high-quality CdSe nanocrystals in noncoordination solvents: “activating agent” and “nucleating agent” controlled nucleation and growth. J Phys Chem C 2009, 113: 8701–8709. 10.1021/jp811308hView ArticleGoogle Scholar
- Empedocles SA, Bawendi M: Spectroscopy of single CdSe nanocrystallites. Acc Chem Res 1999, 32: 389–396. 10.1021/ar9501939View ArticleGoogle Scholar
- Dabbousi BO, Rodriguez-Viejo J, Mikulec FV, Heine JR, Mattoussi H, Ober R, Jensen KF, Bawendi MG: (CdSe)ZnS core-shell quantum dots: synthesis and characterization of a size series of highly luminescent nanocrystallites. J Phys Chem B 1997, 101: 9463–9475. 10.1021/jp971091yView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.